3-D Lanthanide Metal-Organic Frameworks: Structure, Photoluminescence, and Magnetism
Cory A. Black; José Sánchez Costa; Wen Tian Fu; Chiara Massera; Olivier Roubeau; Simon J. Teat; Guillem Aromí; Patrick Gamez; Jan Reedijk; Inorganic Chemistry 48 (2009) 1062–1068; doi:10.1021/ic8017826

data_4301316
_publ_contact_author             'Reedijk, J.'
_publ_contact_author_email       reedijk@chem.leidenuniv.nl
_publ_section_title
;
3-D Lanthanide Metal-Organic Frameworks: Structure, Photoluminescence, and
Magnetism
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1062
_journal_page_last               1068
_journal_paper_doi               10.1021/ic8017826
_journal_volume                  48
_journal_year                    2009
_chemical_formula_moiety         'C42 H57 N9 O18 Tb2'
_chemical_formula_sum            'C42 H57 N9 O18 Tb2'
_chemical_formula_weight         1293.81
_chemical_name_common            'compound 4'
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                101.4720(10)
_cell_angle_beta                 110.5000(10)
_cell_angle_gamma                99.2570(10)
_cell_formula_units_Z            1
_cell_length_a                   10.5390(9)
_cell_length_b                   11.2180(9)
_cell_length_c                   12.8420(11)
_cell_measurement_reflns_used    12617
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      28.74
_cell_measurement_theta_min      1.26
_cell_volume                     1349.0(2)
_computing_data_collection       SMART
_computing_data_reduction        'SAINT (Bruker, 1998)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SIR97 (Giacovazzo et al., 1999)'
_diffrn_ambient_temperature      173(2)
_diffrn_detector_area_resol_mean '8.192 pixels/mm'
_diffrn_measured_fraction_theta_full 0.903
_diffrn_measured_fraction_theta_max 0.903
_diffrn_measurement_device_type  'BRUKER AXS SMART 1000'
_diffrn_measurement_method       omega-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0259
_diffrn_reflns_av_sigmaI/netI    0.0269
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            15867
_diffrn_reflns_theta_full        28.94
_diffrn_reflns_theta_max         28.94
_diffrn_reflns_theta_min         1.76
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.674
_exptl_absorpt_correction_T_max  1.000000
_exptl_absorpt_correction_T_min  0.741671
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker AXS SADABS'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.593
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             646
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.15
_refine_diff_density_max         2.361
_refine_diff_density_min         -1.466
_refine_diff_density_rms         0.124
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.005
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     271
_refine_ls_number_reflns         6447
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.010
_refine_ls_R_factor_all          0.0377
_refine_ls_R_factor_gt           0.0325
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0691P)^2^+1.0232P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0907
_refine_ls_wR_factor_ref         0.0945
_reflns_number_gt                5755
_reflns_number_total             6447
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic8017826_si_002_5.cif
_cod_data_source_block           4
_cod_database_code               4301316